1 TECHNISCHE UNIVERSITÄT MÜNCHEN Physik-Department Lehrstuhl für Funktionelle Materialien Pressure sensitive adhesives - inner structure and adhesive performance Dipl.-Phys. Univ. Markus Schindler Vollständiger Abdruck der von der Fakultät für Physik der Technischen Universität München zur Erlangung des akademischen Grades eines Doktors der Naturwissenschaften (Dr. rer. nat.) genehmigten Dissertation. Vorsitzender: Univ.-Prof. Dr. Martin Zacharias Prüfer der Dissertation: 1. apl.-prof. Dr. Peter Müller-Buschbaum 2. Univ.-Prof. Dr. Friedrich Simmel Die Dissertation wurde am bei der Technischen Universität München eingereicht und durch die Fakultät für Physik am angenommen.
3 Abstract In the presented thesis, the inner structure of acrylic pressure sensitive adhesive (PSA) films comprising of two components is investigated. The main focus lies on the chemical composition in the near-surface region and at the adhesive-adherent interface. The composition at these interfaces is tuned by different post-production treatments of the solution cast adhesive layers and by different cleaning procedures of the adherents. Scattering with x-rays and neutrons allows for structural investigations on the nanometer scale. The inner structure is correlated with the adhesive performance, which is addressed via mechanical probe tack tests. Moreover, a dependency of the failure mechanism during bond rupture on the ambient relative humidity is revealed. The macroscopic tack performance of the PSA and different metals is investigated. The metal film growth on (adhesive) polymer film templates is followed with in-situ x-ray scattering aiming at the metal-adhesive interactions. The near-surface structure formation of diblock copolymers is investigated by in-situ neutron scattering during solution casting, revealing the underlying kinetics details with a resolution on the nanoscale. Zusammenfassung Die innere Struktur von akrylatbasierten, zwei-komponentigen Haftklebstofffilmen (PSA Filme) wird untersucht. Der Hauptfokus liegt dabei auf der lokalen chemischen Zusammensetzung nahe der Oberfläche und an der Grenzfläche zum Substrat. Diese lokalen Zusammensetzungen werden mittels Nachbehandlungen der PSA-Filme, bzw. durch verschiedene Reinigungsverfahren der Substrate, gezielt beeinflusst und eingestellt. Röntgenund Neutronenstreuung ermöglichen eine strukturelle Untersuchung auf der Nanometer- Skala. Korrelationen der inneren Struktur mit dem mechanischen Klebeverhalten, erhalten aus Stempel-Tests, werden aufgezeigt. Eine Abhängigkeit des Versagensmechanismus der Klebeverbindung in Stempel-Tests von der relativen Luftfeuchte wird beobachtet. Das makroskopische Klebeverhalten der untersuchten PSA-Filme in Kombination mit verschiedenen Metallen wird untersucht. Desweiteren wird das Wachstum von Metallschichten auf (adhäsiven) Polymerfilmen mit in-situ Röntgen-Streuexperimenten verfolgt, im Hinblick auf die Wechselwirkungen zwischen Metall und Klebstoff. Die oberflächennahe Strukturbildung von Diblock Copolymeren während des Lösungsgießens wird mittels in-situ Neutronenstreuung untersucht und die zugrundeliegende Kinetik aufgedeckt.
5 Contents Contents iii 1. Introduction 1 2. Theoretical aspects Adhesion Adhesion, cohesion Surface energy, wetting Viscoelasticity Tack test, failure mechanisms Polymer and solvent Statistical copolymers Solubility Scattering methods X-ray reflectivity (XRR) Neutron reflectivity (NR) Grazing incidence small angle x-ray scattering (GISAXS) Grazing incidence small angle neutron scattering (GISANS) Characterization methods Optical microscopy Atomic force microscopy (AFM) Tack-test Contact angle measurements White light interferometry (WLI) X-ray reflectivity (XRR) Neutron reflectivity (NR) Grazing incidence small angle x-ray scattering (GISAXS) Grazing incidence small angle neutron scattering (GISANS) iii
6 iv Contents 4. Sample preparation Investigated polymers Substrate cleaning Deposition methods PSA post-treatments Punch preparation Inner structure and adhesion of the investigated PSAs Topography of solution cast P(EHA-stat-20MMA) films Inner structure of solution cast P(EHA-stat-20dMMA) films Tuning of the near-surface composition of P(EHA-stat-20MMA) Surface enrichment of EHA Surface enrichment of MMA Tackiness and failure mechanisms Tuning of the adhesive-adherent interface composition Vertical structure evolution in films of P(EHA-stat-20dMMA) Autoadhesion of PMMA Autoadhesion under high humidity Autoadhesion under low humidity Summary Metal-adhesive interactions Adhesion of metals on P(EHA-stat-20MMA) Surface energies Tack performance Metal film formation upon sputtering Aluminum deposition Gold deposition Growth model Summary Structure formation of block-copolymers during drying P(dS-b-nBMA) in toluene Structure formation followed by in-situ neutron reflectivity Solvent loss during drying Dry state investigated by TOF-GISANS
7 Contents v 7.2. P(dS-b-nBMA) in dimethylformamide Structure formation and solvent loss followed by in-situ neutron reflectivity Structure formation followed by in-situ TOF-GISANS TOF-GISANS goes reflectivity Summary Conclusion and outlook 133 Appendices 137 A. Contact angle measurements 139 Bibliography 143 List of publications 162 Acknowledgements 167
9 1. Introduction The application of adhesives has already a long history. While up to the 19th century glues were made of plants and animals, the fabrication of adhesives is nowadays almost entirely based on synthetic chemicals . As long as their history as wide is the range of applications for adhesive bonding. Many kinds of industries, for instance in the automotive or aircraft production, have already replaced their traditional ways of joining workpieces like welding or riveting by adhesive bonding. Examples of the major advantages of this kind of joining are for instance the resulting weight and cost reduction as well as the omitted need of structural weakening of the work pieces. Also human beings are subjects to adhesive bonding, e.g. in case of dental treatments . Everyday-life applications of adhesives are often found to exhibit a moderate bonding strength for bond-and-release tasks like medical patches, duct tape or sticky notes. These examples are representatives of the class of pressure sensitive adhesives (PSAs). A strength of adhesives in general is the ability to join very different kinds of material, e.g. glass, paper, wood or metal . PSAs are used for the immediate and also permanent bonding to almost any surface even under small pressure [4, 5, 6]. This feature of immediate adhesive bonding without the need of solvents is in literature also referred to as instantaneous adhesion or quick stick . The reason for their variability lies also in the chemical nature of the involved polymers, with acrylates, rubbers and silicones being prominent representatives . The attractive forces leading to adhesive bonds using PSAs are typically van der Waals forces. Therefore, no chemical reaction, melting or solvent evaporation are involved in the bond formation. The adhesive joint sustains a certain level of stress before the bond ruptures. This process of debonding is rather complex due to the dissipation of energy via plastic deformation and mechanical failure of the adhesive. Therefore, an adhesive must be balanced in terms of adhesive and cohesive strength . A complete understanding of the physical processes during debonding has not been achieved so far, because the deformation of viscoelastic adhesives involves highly nonlinear effects. Moreover, due to the ability to be tuned to the desired needs by certain additives, PSAs are usually comprised of more than one component, which leads to an almost arbitrarily high complexity of the system. Some implications can be phase separation or inhomogeneous spatial distributions of the different components in the additive. 1
10 2 Chapter 1. Introduction Among the different types of PSAs already mentioned above are acrylate based PSAs, which are investigated in this thesis. They typically consist of statistical copolymers, in which the two kinds of monomers fulfill the desired needs concerning adhesive and cohesive properties . Block copolymers are more rarely used, but still are used in specific applications. In this work the PSAs consist of the monomers ethylhexylacrylate (EHA) being the soft and sticky component and methylmethacrylate, representing the glassy and stiff material. Commercial PSAs include many additives which are chosen on an empirical trial-and-error basis which is faster and cheaper than investigations of the involved fundamentals. Consequently, a deeper understanding of the influence of the involved additives exhibits only a slow progress. For an unambiguous interpretation of the performed structural and mechanical investigations, this work is focused on two-component systems. The adhesive performance of such model systems for PSAs has already been investigated in literature [10, 11, 12]. Also the near-surface composition has been addressed by x-ray reflectivity , recently. The present work adds the investigation of i.a. the composition of the PSA in vicinity of the adhesive-adherent interface. The local composition at this buried interface is of utmost importance for possible predictions concerning duration and strength of the adhesive bond. The probe to access this adhesive-adherent interface are neutrons, which are able to penetrate both adhesive and adherent up to large depths. The methods of choice for investigations of this kind are neutron reflectivity (NR) and grazing incidence small angle neutron scattering (GISANS). While NR provides insights into the composition profiles of layered structures, GISANS offers in addition the information about i.a. the size of lateral structures. After introducing the theoretical background of this thesis (chapter 2) the experimental methods used are detailed in chapter 3. Subsequently, the sample preparation is addressed in chapter 4. Figure 1.1 summarizes the different aspects dealt with in the present thesis. These projects are briefly explained in the following. Chapter 5 provides insights into the inner structure of the model PSA poly(ethylhexylacrylate-stat-20 methyl methacrylate) and its adhesive performance (figure 1.1a). The main focus in this chapter is on the inner structure of the PSA film at and close to the surface and also at the adhesive-adherent interface. The question to answer is: If and how does the inner structure affect the adhesive performance? Moreover, to what degree can the performance be tuned to the desired needs? For this purpose post-production treatments with different relative humidities are applied. Also, the autoadhesion of poly(methyl methacrylate) is addressed in this chapter, which is of high interest e.g. for crack healing in polymeric materials. Chapter 6 deals with a common adhesive application in industries, the adhesive joining of
11 3 Figure 1.1.: Overview: The inner structure of a model pressure sensitive adhesive is investigated and related to its adhesive performance. Among the different techniques applied for this task are the three techniques depicted in a: Atomic force microscopy, neutron reflectivity and tack test. To investigate the bonds of metal and the model PSA (b), tack tests are performed. The metal growth on adhesive films is investigated with in-situ grazing incidence small angle x-ray scattering. Insights into the structure formation in polymer films upon solution casting are obtained by in-situ investigations of the structural evolution during drying of diblock copolymers (c). The applied techniques are neutron reflectivity and grazing incidence small angle neutron scattering. metal work pieces (figure 1.1b). This goal can in principle be achieved by two approaches. At first, an adhesive layer can be applied on a metal surface, which is the most common case. Therefore, the tack performance of the model PSA in combination with different metal adherents is investigated. The obvious question is: How does the adhesive performance depend on the chosen metal? In another approach, the metal layer is grown on the already pre-existing adhesive polymer film. Therefore, the metal film growth and the inner structure of the metal layer are also investigated in this chapter to find out how metal films grow on different polymer templates. Finally, in chapter 7, the structure formation of diblock copolymers during solution casting is investigated (figure 1.1c). For the first time, in-situ GISANS measurements are successfully performed at the liquid-air interface.
13 2. Theoretical aspects In this chapter the key-factors for the establishment of adhesive bonds are explained. At first, van der Waals forces are introduced, which are the most relevant forces in adhesive bonding using pressure-sensitive adhesives. Subsequently, the theoretical background of surface tensions (also called surface energy) and wetting of surfaces is explained. Furthermore, the polymer-specific feature of viscoelasticity is described, along with a theoretical treatment of the tack-test. This method is used in this work to investigate the adhesive performance of a model PSA and reveals the different failure mechanisms of the adhesive bonds. These mechanisms are also addressed in this chapter. The inner structure of polymers in general and in particular of PSAs, as well as the structural evolution, are mainly governed by polymer-polymer and polymer-solvent interactions. Therefore, these interactions are also dealt with in this chapter. Scattering techniques, utilizing both x- rays and neutrons, are applied to obtain information about the spatial composition of the individual components in the polymer films on the nano-scale. While reflectivity measurements yield information about layered architectures in perpendicular direction to the sample surface, grazing incidence techniques are capable of detection and quantification also of lateral structures. The theoretical background for these techniques is explained in the end of this chapter Adhesion In this section the theoretical background of adhesion is addressed. Starting from van der Waals forces, the fundamental forces responsible for the adhesion of PSAs, the main factors which influence the strength of an adhesive bond are explained. At first, the theory of surface tension and surface wetting is detailed. The polymer-specific phenomenon of viscoelasticity is subsequently addressed, before this section concludes with the theory of the tack-test and an overview over different failure mechanisms, which can occur during the debonding of an adhesive joint. 5
14 6 Chapter 2. Theoretical aspects Adhesion, cohesion In the case of PSAs the ability to establish adhesive bonds is mainly due to Van der Waals forces . Other possibilities for adhesive joints without chemical reactions taking place can be of electrostatic nature or based on diffusion and polymer chain entanglement (see also section 5.6) . Van der Waals forces can be categorized in three different kinds of interactions [1, 15]. The Keesom energy is derived from the attraction of two permanent dipoles µ 1 and µ 2 with a distance r and results in equation (2.1), µ µ 2 E Keesom = 3(4πǫ 0 ) 2 k B Tr6, (2.1) ǫ 0 being the dielectric permittivity in vacuum, k B the Boltzmann constant and T the temperature . For only one permanent dipole and another molecule with polarizability α, the permanent dipole can induce an additional dipole moment in the second molecule. This interaction is called Debye interaction which leads to the energy relation in equation (2.2) . E Debye = µ2 α (4πǫ 0 )r6. (2.2) The third van der Waals force results from two polarizable molecules. A spontaneous dipole moment is created in the first molecule via fluctuations in the electron shell. This induces a dipole in the second molecule and results in an attractive force. The corresponding energy is called London energy: E London = 3(α 1α 2 ) 2 I 1 I 2 2(I 1 +I 2 )r 6, (2.3) with I i being the ionization potentials of both molecules . Due to the proportionality of all three contributions to r 6 they can be written in a single term with one contribution of each interaction: E vdw = C Keesom +C Debye +C London r 6 = C vdw r 6. (2.4) At very small distances the Pauli principle takes effect  and outweighs the attractive forces. Therefore, two molecules cannot approach each other to an arbitrary vicinity due to the resulting repulsive potential. The total potential, taking van der Waals forces and the Pauli principle into account, is called Lennard-Jones potential  (see equation (2.5)). E Lenard Jones = C Pauli d 12 C vdw d 6 (2.5)
15 2.1. Adhesion 7 Figure 2.1: a) Work of adhesion: Separation of materials A and B from contact to infinite distance. b) Work of cohesion: Separation of two parts of the same material A from contact to infinite distance. The thermodynamic work of adhesion W Adhesion is defined as the work necessary to separate two materials in contact to an infinite distance (see figure 2.1) . This quantity is entirely thermodynamic which means it does not account for energy dissipation in form of e.g. deformation and therefore is not to be mixed up with the tack energy obtained from tack measurements (see chapter 2.1.4). To separate two materials of the same kind the work of cohesion W Cohesion is necessary  Surface energy, wetting The surface energy or surface tension γ A is defined as the energy E needed to increase the surface area A of a material by its unit area (2.6): γ A = E A. (2.6) From the cohesion point of view the surface area of a material A can be increased by splitting it into two parts (see figure 2.1 b) and the surface energy can be written as γ A = 1 2 W AA. (2.7) Incaseofadhesion, wheretwoimmisciblematerialsaandbgetincontact, thefreeenergy is minimized by a change in interfacial area. The resulting interfacial energy resembles the corresponding free energy change per unit area and is referred to as the Dupré equation  γ AB = 1 2 W AA W BB W AB = γ A +γ B W AB. (2.8) In practice, the Dupré equation is used for liquid-solid interfaces and therefore reads γ SL = γ S +γ L W SL. (2.9) This situation can be discribed using the Young and Young-Dupré equations : Young-Dupré equation: γ B (1+cos(Θ)) = W AB (2.10)
16 8 Chapter 2. Theoretical aspects Figure 2.2.: A liquid (L) wetting a solid (S) under ambient conditions (V). Θ denotes the contact angle. Young equation: γ AB +γ B cos(θ) = γ A. (2.11) Equation 2.10 yields the work of adhesion of a liquid droplet on a solid substrate based on the contact angle and the surface energy of the liquid. The Young equation (equation 2.11) provides means to access the interfacial energies from known single surface energies and a measured contact angle. The work of adhesion does not enter in equation An important prerequisite for strong adhesive bonding is proper wetting, which means thatthecontactangleθbetweenadhesiveandadherentneedstofulfillθ 90 (seefigure 2.2). More detailed discussions about wetting, its statics and dynamics and major impact factors can be found in [14, 21, 22, 23, 24]. To derive the surface energies of a given solid, Owens and Wendt  used the Young equation, knowing the surface tensions of a set of test liquids. These surface tensions were deduced from contact angle measurements on the solid specimen. This approach is based on the postulation that a surface tension can always be described as the sum of a dispersive and a polar part . The London forces are the origin for the dispersive contribution, while the Keesom and Debye forces determine the polar part (see section 2.1.1). For an exemplary liquid L on a solid S this approach reads γ L = γl d +γ p L and γ S = γs d +γ p S. (2.12) The relation to the solid-liquid interfacial tension becomes γ SL = γ S +γ L 2 γ ds γdl 2 γ p S γp L, (2.13)
17 2.1. Adhesion 9 and by the use of the Young equation, equation 2.14 can be derived : γ d 1+cosΘ = 2 γs d L γ p +2 γ p L S. (2.14) γ L γ L For clarity the subscripts for the liquids can be skipped and only the solid under investigation is subscripted in the following. Equation 2.14 can be rewritten as a linear equation: (1+cos(Θ))γ γ 2 = γ dsolid γ + γ p d solid 1. (2.15) γd This linear equation has a slope γ p solid and an intersection with the y-axis at γ d solid. All terms are known, except the contact angle Θ, which is the quantity to be measured. This non-destructive method to derive the dispersive and the polar part of the surface tension via contact angle measurements is called Owens-Wendt method. Six different test liquids are used in this work to improve the accuracy of the resulting surface tension. A linear fit to the six measured data points was done to minimize the measurement uncertainty Viscoelasticity The strength of a successfully installed adhesive bond depends also on the ability of the adhesive to dissipate energy while debonding, meaning sustaining a certain level of stress . In PSAs this is usually realized via mechanical deformation. Viscoelasticity is an unique property of polymers and applies especially to PSAs. So-called creep experiments can be carried out to address this feature . In these experiments, a force is instantaneously applied to the specimen and the time dependent deformation of the polymer is measured. This elongation is commonly normalized to the original sample length to obtain the time-dependent longitudinal strain ǫ(t). After a time t, the force is removed and the recovery process of the specimen can be followed. Considering sufficiently small applied forces the reaction of the polymer can be described by linear equations. Figure 2.3 schematically shows possible results for the strain for an uniaxial applied tensile load. It is obvious that viscoelasticity is not just a superposition of viscocity and elasticity, but comprises also a phenomenon called anelasticity. An elastic specimen under an applied constant force follows Hook s law (figure 2.3a), while a material exhibiting viscous flow undergoes permanent deformation accompanied by stress relaxation (figure 2.3b). The behavior of a viscoelastic polymer is shown in figure 2.3c, where the anelastisity can be observed as a retarded elasticity. The time-dependent longitudinal strain ǫ(t) can be specified more precisely ǫ(t) = ǫ zz (t). The first index refers to the direction of the normal vector of the surface on which the force acts upon. The second index denotes the direction of the stress component . By normalizing the acting force to the area it is
18 10 Chapter 2. Theoretical aspects Figure 2.3.: Longitudinal strain evolution versus time for different behaviors: a) elasticity, b) viscosity, c) viscoelasticity. acting on, a constant tensile stress σ 0 zz is derived. Finally, the tensile creep compliance D(t) = ǫ zz (t)/σ 0 zz can be introduced . Another approach to access the viscoelastic properties is the stress relaxation experiment. In this method a constant tensile strain ǫ 0 zz is imposed to the specimen and the time dependent stress σ zz (t) is measured. Thereby, the tensile modulus Ẽ(t) = σ zz(t)/ǫ 0 zz is obtained . In a third kind of experiment a periodically varying stress field σ zz (t) = σ 0 zzexp[ iωt] is applied. The resulting strain reads  ǫ zz (t) = ǫ 0 zzexp[iφ]exp[ iωt]. (2.16) The dynamic tensile compliance D(ω) and along with it the dynamic tensile modulus Ẽ(ω) follow: D(ω) = ǫ zz(t) σ zz (t) = D +i D (2.17) Ẽ(ω) = ( D(ω) ) 1 = Ẽ +iẽ. (2.18) In applications the dynamic shear modulus G(ω) of PSAs is of utmost importance and therefore experiments usually adress this quantity : G(ω) = σ zx(t) ǫ zx (t) = σzxexp[ iωt] 0 ǫ 0 zxexp[iφ]exp[ iωt] = σ0 zx exp[ iφ] = ǫ G (ω)+i G (ω). (2.19) 0 zx G isreferred to asstoragemodulus and G asloss modulus. G isthe quantityresponsible for the energy exchange in dynamic experiments, whereas G gives information about the dissipated power. Due to the fact that the described dynamic measurements do not deliver the same amount of information as creep or stress relaxation measurements, they are not onlyperformedatonesinglefrequencyω,butinrangesoveruptofourordersofmagnitude . To even enlarge this still limited range, these experiments are carried out at different temperatures, which further completes the knowledge of the viscoelastic behavior of the specimen. The measurements carried out at different temperatures, each across a broad
19 2.1. Adhesion 11 Figure 2.4: Rheological data for poly(ethylhexylacrylate) (PEHA): E denotes the storage modulus, E denotes the loss modulus. Timetemperature superposition was applied to obtain a master curve. The image is taken from . frequency range, are then combined using a temperature-dependent shift factor to obtain the so-called master curve . Exemplary master curves for storage and loss moduli are shown in figure 2.4. The data was collected for the homopolymer poly(ethylhexylacrylate), a standard component in model PSAs, with a parallel plate shear rheometer using a spectrum of temperatures and frequencies which were then combined via time-temperature superposition to obtain the master curves  Tack test, failure mechanisms The most important property of an adhesive is the ability to form bonds of a desired strength between different kinds of materials. In particular the class of PSAs is capable of joining very different materials such as paper, wood or metal [3, 10]. To test the performance of an adhesive many mechanical tests are used, which mimic certain applications of the adhesive to account for e.g. mechanical deformation. Well established examples are the rolling-ball-test [31, 32], rolling cylinder test , peel-test [34, 35], Johnson-Kendall- Roberts method , the tack [3, 37, 38] and the loop tack test  and finally the finger  and the shear adhesion test . For adhesion measurements on the nano scale the atomic force microscope (AFM) is the method of choice [42, 43] which is sensitive even to friction and rupture of single polymer chains . For scientific approaches and systematic investigations the probe tack test offers several advantages which make this method superior to others and which will be explained in the following. In a tack test (see figure 2.5) a cylindrical probe of radius r is pressed onto an adhesive layer of thickness h for a given time period t and thus creates a nominal stress σ N (figure 2.5b). Subsequently, the punch is retracted at a constant rate v and the necessary force F is recorded as a function of the distance to the sample surface d (figure 2.5c). The outcome of such a tack experiment is the corresponding tensile stress σ zz as a function of the distance d. For
20 12 Chapter 2. Theoretical aspects Figure 2.5.: Principle of a tack measurement: a) The punch with radius r approaches the PSA film (thickness h). b) The punch and the PSA are kept in contact by applying a pressure for a certain time. c) The punch is retracted and a force-distance curve is recorded. probing the PSA different punch tip geometries are possible, e.g. spherical or flat ended . The spherical punch provides better reproducible results by a reduced sensitivity to alignment and is therefore mostly used in industry. The geometry used in this work is the flat-ended cylinder, which results in a homogeneous stress distribution in the PSA and consequently a homogeneous debonding. Furthermore, this work is focussed also on the near-surface region of the PSA, up to 100 nm in depth. To be able to probe regions of this depth and smaller, a flat-ended punch is crucial due to its high surface sensitivity. For an unambiguous interpretation of the obtained tack results it is required that the bond between the PSA and its substrate is stronger than the bond between PSA and punch probe, so that only the surface-near region of the PSA is probed in the experiment. The stress field in the adhesive layer below the punch is a function of the ratio α = r/h, which is referred to as the confinement . This stress field can only be calculated via finite element methods . For large values of α however, the pressure distribution p(r) is found to be parabolic  ( ) p(r) = σ zz (r) = p 0 2λσ N 1 r2, (2.20) a 2 with r being the radial distance from the symmetry axis, p 0 the external (usually atmospheric) pressure, λ = (h+d)/h the extension ratio, σ zz the normal and σ N the nominal tensile stress. σ N is derived from the tensile load P by σ N P/(πr 2 ). For an incompressible elastic solid the nominal stress reads σ N = 8Gd πr. (2.21) For even a slight deviation from incompressibility the stress field below the probe punch becomes rather flat . This is experimentally evidenced by the fact that in case cavitation occurs, it is observed simultaneously over the whole surface of the probe .